NUCLEATION AND GROWTH BEHAVIORS OF PRI-MARY PHASE IN AL-CU HYPEREUTECTIC ALLOY IN HIGH MAGNETIC FIELDS
C. Li, Z. Ren, W. Ren, Y. Wu, Y. Zhong, and K. Deng
School of Materials Science and Engineering and Shanghai Key Laboratory of Modern Metallurgy & Materials Processing Shanghai University
Shanghai 200072, China
Abstract—The nucleation and growth of primary Al2Cu phase in the
Al-34.3wt%Cu hypereutectic alloy without and with magnetic fields have been investigated by differential thermal analysis (DTA). The DTA curves indicated that the nucleation temperature of primary phase was significantly reduced in a magnetic field. The X-ray diffraction (XRD) patterns confirmed that thec-axes of primary Al2Cu
crystals oriented along the direction parallel to a magnetic field. The microstructures showed that primary crystals aligned along a magnetic field and that their number distinctly increased with increasing a magnetic field as well. The suppression of nucleation in a magnetic field could be caused by the increase of the interfacial energy between the liquid and nucleus and the reduction of atom diffusion rates while the orientation of primary crystals were mainly attributed to both of the magnetic torque and the thermoelectric magnetohydrodynamic (TEMHD) flows.
In recent decades, numerous new phenomena successively have been found in the materials processing by applying a high magnetic field. Among these phenomena, magnetic orientation has attracted many scientists. It is well-known that crystals with magnetic anisotropy can orient in a magnetic field, and therefore a high magnetic field has been widely used to prepare materials with oriented structures. As early as 1930s, Goetz  found that a magnetic field could induce
Received 13 June 2010, Accepted 2 September 2010, Scheduled 21 October 2010
orientation in producing Bi single crystals. By the 1980s, Mikelson and Karklin  observed that the oriented structures were obtained in a series of alloys like Al-Cu alloys in a magnetic field. Savitisky et al.  found that ferromagnetic MnBi phase could orient along magnetic force lines in solidification experiments. Then, Rango et al.  succeeded in preparing bulk texture samples of YBa2Cu3O7. Recently, many
studies have concentrated on the effect of magnetic fields on oriented structures of superconducting materials , magnetic materials , nano materials , and even biological materials . More recently, Tournier and Beaugnon  reviewed texturing by cooling a metallic melt in a magnetic field and pointed that texturing from a melt was successful when the overheating temperature was just a few degrees aboveTm and failed when the processing time aboveTm was too long or when the overheating temperature was too high. Based on the experimental results, they thought that intrinsic solid nuclei existed in the melt and proposed a model that predicts the existence of unmelted crystals above the melting temperature Tm .
Nevertheless, to authors’ knowledge, there are few studies on the effect of a magnetic field on the nucleation and growth behaviors of oriented phase, both of which, without a doubt, play an important role on the formation of texturing in a magnetic field. In addition, no research pays attention to the process that oriented structures evolve accompanying crystal growth though it is well known that the crystal with susceptibility anisotropy in the weak constraint medium can rotate and orient on the action of a magnetic field. Thus, the work aims to investigate nucleation and growth of primary Al2Cu phases
in the Al-Cu hypereutectic alloy in a magnetic field by differential thermal analysis (DTA) in order to deeply understand the formation of oriented structures. A new explanation on formation mechanism of aligned crystals in a magnetic field has been proposed.
2. EXPERIMENTAL DETAILS
The DTA apparatus was used to detect the solidification behaviors of the alloy, which was described in detail in previous work . The whole equipments mainly consisted of superconducting magnet (Oxford Instruments), DTA apparatus, programming controller and model 2700 (Keithley Instruments, Inc.). The magnet can produce a magnetic field with a maximum intensity up to 14 T. In experiments, the samples in the DTA apparatus were placed in the center of magnet, namely, the position of the maximum intensity of a magnetic field.
analysis showed the alloy with a composition of Al-34.3wt%Cu. The cylindrical samples with a diameter of 4 mm and a height of 4 mm for DTA were obtained by wire cutting. The DTA tests were carried out in a temperature range from a room temperature up to 700◦C. The
samples were heated to 700◦C at the rate of 10◦C/min, hold for 20 min
and then cooled at the rate of −5◦C/min. The heating chamber was
fluxed with high pure argon in runs.
The post-treated samples were cut along the directions parallel and perpendicular to a magnetic field. The microstructures of samples on different sections were examined by using an optical microscopy after mechanically polishing and etching. The crystallographic orientation was studied by X-ray diffraction (XRD) with Cu-Ka.
In order to detect the effect of a magnetic field on nucleation of primary phase in the Al-34.3wt%Cu alloy, the DTA tests have been carried out with and without magnetic fields at the cooling rate of−5◦C/min. As
showed in Figure 1, two exothermic peaks are readily observed on each DTA curve. Minor peaks originate from the precipitation of primary Al2Cu crystals and the major ones are from the growth of Al-Al2Cu
eutectics. The nucleation temperatures Tn of primary Al2Cu crystals
in magnetic fields are obviously lower than that without a magnetic field. The nucleation temperature in 12 T magnetic field even is about
480 500 520 540 560 580 600
0T 2T 6T 12T 4o
Figure 1. DTA curves of the Al-34.3wt%Cu alloy at cooling rate of −5◦C/min. The nucleation temperature T
0 20 40 60 80 100 B=0T
2 Theta (deg.)
(110 ) (220 ) (112 ) (310 ) (330) (311 ) (224 ) ο ∆ Al2Cu
Al (220 ) (111 ) B=12T
0 20 40 60 80 100
B=0T Intensity, a.u. (400) (311) (200) (111) (110) (002) (004)
ο ∆ ο ∆ ∆ ∆ ∆ ο ∆ ο ∆ ο ∆ ∆ ∆ ο ο ο
2 Theta (deg.)
Figure 2. X-ray diffraction patterns of the samples obtained with and without the applied magnetic field of 12 T on (a) longitudinal and (b) transversal sections.
8◦C below that without a field. It demonstrates that a magnetic field suppresses the nucleation of primary phase in the melt. Moreover, the nucleation temperature is reduced as a magnetic field increases. It means that it is more difficult for primary Al2Cu crystals to nucleate in the melt in higher magnetic field.
The XRD patterns of the samples obtained with and without a 12 T magnetic field are displayed in Figure 2. All the (h k l) peaks with zero l values of Al2Cu crystals on the longitudinal section of samples
appear in the presence of a magnetic field in comparison with those without a magnetic field, as showed in Figure 2(a). XRD patterns on the transversal sections show (0 0l) peaks of Al2Cu crystals either
appear, e.g., (0 0 2), or are enhanced, e.g., (0 0 4) in a 12 T magnetic field. Thus, the XRD patterns clearly confirmed that the c-axes of Al2Cu crystals oriented along the direction parallel to a magnetic field.
(e) B (f) B
(g) (h) B
Figure 3. Microstructures of the Al-34.3wt%Cu alloy at cooling rate of −5◦C/min with and without magnetic fields. (a) Longitudinal,
(a)0T (b)6T (c)12T
Figure 4. Three dimensional diagram of microstructures of Al-34.3wt%Cu alloy in different magnetic fields.
magnetic field increases (Figures 3(d), (f) and (h)) in comparison with those without a field (Figure 3(b)). It signifies that the number of critical nuclei of primary phase from the melt increases in a magnetic field. The results are in good agreement with the reduction of nucleation temperature Tn of primary phase in the DTA tests.
In order to distinctly show the orientation of primary phase in samples, we constructed three dimensional diagrams of microstructures of Al-34.3wt%Cu alloy, as showed in Figure 4. From the pictures, one readily obtains the spatial distribution of oriented primary phase. Obviously, most primary crystals orient along a magnetic field and grow to elongated shapes in magnetic fields of 6 T and 12 T (Figures 4(b) and (c)).
From the above results, a magnetic field significantly influences the nucleation, e.g., reduction of nucleation temperature, and growth of primary phase, e.g., orientation.
Firstly, let us consider the nucleation in a magnetic field. In the classical nucleation theory, the difference of bulk Gibbs free energy between the liquid and crystal phases and the interfacial energy together determine activation energy of nucleation. The activation energy ∆G∗ can be written as 
In the Equation (1), ∆GV is the difference in bulk Gibbs free energy, γsl is the solid-liquid interfacial energy and f(θ) is catalytic factor.
Gibbs free energy induced by a magnetic field is extremely subtle for non-magnetic materials according to Magomedov’ report , which can be ignored compared with bulk Gibbs free energy. Additionally, although only minor undercoolings were obtained in the course of solidification in the present experiments, there was no reason to believe that a magnetic field changed catalytic factor in the same experimental conditions, such as crucible walls, inclusions, except a magnetic field. However, as we know, the interfacial energy is closely related to undercooling and even their relation was used to calculate the solid-liquid interfacial energy in the case of maximum undercooling . Thus, it is inferred that a magnetic field changes the interfacial energy between the liquid and nucleus and further alters the activation energy for nucleation according to the change in nucleation temperature. There were some reports showing that a magnetic field could change the interfacial energies of some substances, e.g., water , pure aluminum . For the Al-Cu alloy, moving Al and Cu atoms in the melt will be subjected to the Lorentz force in a magnetic field, which causes unstable atoms on the interface to migrate to a more stable position . It may be said that it is more difficult for atoms to attach themselves to a nucleus. According to definition of interfacial energy that the work dW required to create a new area dA of interface is dW =γdA, more energy, dW, is needed to form a new interface by increasing the number of atoms on the interface, namely, the interfacial energy should be increased in a magnetic field. In addition, another factor should be considered, i.e., atom diffusion. For solidification of alloys, as Turnbull pointed out , long-range diffusion was to be expected in phase transformations that involve more than one component. The activation energy for diffusion was determined by the most slowly moving component. There are a number of reports showing that a magnetic field could effectively suppress the atom diffusion in the conducting liquids [19, 20] and alloys . On the one hand, a magnetic field suppresses the convection of the melt and the mass transfer is mainly dominated by atom diffusion rather than convection. On the other, a magnetic field reduces the diffusivity of solute atoms in the melt. This means that activation energy for diffusion increases in a magnetic field. The change of the diffusivity and attachment kinetics in a magnetic field leads to increase the nucleation barrier and delay the formation of critical nuclei. Hence, the undercooling correspondingly increases in a magnetic field, which is characterized as the reduction of nucleation temperature Tn.
depends on the magnetic properties of a crystal in order to keep the lowest magnetic energy. The magnetic energy of the grain in a magnetic field can be expressed as following 
Em(θ, H) =−V H
χab+ ∆χcos2θ¢ (2) In the Equation (2), ∆χ = χc − χab, where χc is magnetic susceptibility along c-axis. χab is the susceptibility in the a or b-axis direction. V is the volume of the grain, H is a magnetic field, θ is the angle between a magnetic field andc-axis. For the Al2Cu crystal, it has a tetragonal structure. From XRD diffraction patterns, it can be concluded that the Al2Cu crystal possesses magnetic anisotropy
and its magnetic susceptibility χab is lower than χc. Therefore, the
c-axis of the Al2Cu crystal orients along a magnetic field due to Em(0, H)< Em(π/2, H).
Nevertheless, the magnetic torque, on one hand, compels the c -axis with the maximum susceptibility of primary tiny crystals to rotate to the direction parallel to a magnetic field. On the other hand, the thermal energy disturbs the rotation of tiny crystals in the melt. As primary phases grow, the magnetic energy will exceed thermal energy. The condition can be read as ,
|∆E|> kT (3)
where ∆E is magnetic energy difference between mutually perpendic-ular axes. k is the Boltzmann constant. If we insert the expressions
Em(0, H) andEm(π/2, H) into Equation (3), then 1
2> kT (4)
From Equation (4), the magnetic energy difference increases as the grain grows and finally exceed the thermal energy. In the case, the crystal succeeds to rotate and orient. Moreover, the time for rotation is extremely short, such as, the time is about 1ms in a magnetic field of 10 T . It is assumed that the grain is spherical and its radius is
rc when the magnetic energy difference is equal to the thermal energy. From the preceding analysis, when the radius of tiny crystals r is less than rc, the magnetic field cannot overcome thermal energy and thus the grain does not orient or vice versa.
Step 1 Step 2 Step 3
Figure 5. Schematic diagram of formation of an elongated primary phase in a magnetic field.
embryos. The magnetic torque M for a crystal in a homogeneous magnetic field can be expressed as following:
M = ∆χB2V
2µ0 sin 2α (5)
where α is the angle between a magnetic field B and the axis with maximum susceptibility. From the Equation (5), the higher a magnetic field, the larger the magnetic torque. Therefore, the degree of orientation should be higher as a magnetic field increases. This has been testified from longitudinal microstructures in magnetic fields, as showed in Figure 3. However, it can be imagined that tiny crystals in shape from the melt initially do not exhibit elongated Al2Cu
crystals along a magnetic field although the shape anisotropy is also an important factor for the orientation of crystals because the formation of resulting elongated primary crystals depends on growth kinetics. It may be inferred that the change of growth rates in different directions in a magnetic field leads to the formation of the elongated primary phases. Consequently, the elongated primary crystals can be achieved through three steps below and the forming progress of oriented crystals can be illustrated as displayed in Figure 5.
Step 1: Critical nuclei with radius r∗ form in the melt as the
Step 2: Tiny crystals with radius rc > r∗, which nuclei grow to, succeed to rotate and orient in the condition that the magnetic energy is larger than the thermal energy.
phase finally grow to the elongated crystals.
The first two steps have been discussed in preceding section. How does a magnetic field affect the growth rates in the different directions? We discuss how the grains grow to the elongated crystals in a magnetic field as following.
It is well known that the rates of crystal growth are mainly governed by heat and mass transfer. Primary phase can grow more quickly in the directions where the diffusivities of heat and atom are larger. In the absence of a magnetic field, the sample more quickly dissipated heat in the radial direction as the furnace temperature fell. Consequently, primary phase tended to grow along the radial direction (Figure 3(a)). Nevertheless, when applying a magnetic field, the rates of radial heat loss could be reduced since a magnetic field effectively suppressed thermal convection . Radial growth became slow accordingly. Additionally, although convection of electrically conducting melt could be damped by a magnetic field in macroscopic scale , the thermoelectric magnetohydrodynamic (TEMHD) flows in micro scale exerted an appreciable effect on crystal growth . Much research work fully demonstrated that the TEMHD flows induced by a magnetic field played an important role on solidification of metallic alloys. Moreau et al.  found that an external magnetic field could cause TEMHD flows around dendrites during solidification of the Bi-Sn alloy. Gorbunov  first investigated the effect of TEMHD on single crystal growth. Li et al.  observed that TEMHD flows had a marked effect on interface shape and cellular morphology during directional solidification and evaluated the magnitude of the flows at different scales.
In the growth of primary Al2Cu crystals, the temperature gradient appears near the solid-liquid interfaces due to latent heat release. The thermoelectric currents j can be produced when the gradients of thermoelectric power S and temperatureT are not parallel. It can be read as 
where σ is electrical conductivity of the material, ∆S is the thermoelectric power of the metal pair, ∇T is the temperature gradient. The interaction between an applied magnetic field and a thermoelectric current generates a thermoelectric forceF, which drives a TEMHD flow.
F =−σ∆S∇T×B (7)
Following Li et al’s evaluation , The TEMHD flows dominate the convection of the melt when the magnetic field is less than the critical magnetic fieldBmax. It can be expressed as following
Bmax= L1 ³µ
where L is characteristic length, µ is the dynamic viscosity. In the current experiments, the typical values for Al-Cu alloys are listed below: L = 1µm, µ(700◦C) = 1.15×10−3Pa·s , σ(700◦C) =
3.0 × 106Ω−1m−1 , ∇T = 10 K · cm−1. Substituting these
parameters into the Equation (8), one easily deduces that the value of Bmax is about 19 T. Obviously, the applied magnetic fields (12 T)
are less than 19 T. Thus, the thermoelectric force can drive the flows of the melt beyond the magnetic damp on micrometer scale. According to the relation between directions of thermoelectric currents and a magnetic field, one readily obtain directions of thermoelectric force and TEMHD flows, as showed in Figure 6(a). From the picture, the TEMHD flows continually sweep the solid-liquid interface, which make it more difficult that solute atoms deposit to a crystal. The amplitude of TEMHD flows near lateral interfaces is relatively larger than that on others owing to a vertical magnetic field. Hence, the rates of crystal growth inx-direction are slower than those inz-direction, as displayed in Figure 6(b). The TEMHD flows, therefore, change the rates of atom deposition, i.e., growth rates, on different positions of the interface. The primary phase finally grow up to the elongated crystals along a magnetic field.
Al-34.3wt%Cu. The DTA curves showed that the nucleation of primary phase was markedly suppressed in magnetic fields, which was further demonstrated by the increase of the number of primary crystals on the transversal sections. The suppression of nucleation could be attributed to the increase of interfacial energy and the reduction of diffusion rates while the magnetic torque and the TEMHD flows were responsible for the formation of oriented crystals.
The authors are grateful for the financial support of Natural Sci-ence Foundation of China (Grant Nos. 50911130365, 50701031, IRT0739), Science and Technology Committee of Shanghai (Grant Nos. 09510700100, 08dj1400404, 08DZ1130100) and China Postdoc-toral Science foundation (Grant No. 20090450686).
1. Goetz, A., “On mechanical and magnetic factors influencing the orientation and perfection of bismuth single-crystals,” Physical Review, Vol. 35, 193–207, 1930.
2. Mikelson, A. E. and Y. K. Karklin, “Control of crystallization processes by magnetic fields,”Journal of Crystal Growth, Vol. 52, 524–529, 1981.
3. Savitsky, E. M., R. S. Torchinova, and S. A. Turanov, “Effect of crystallization in magnetic field on the structure and magnetic properties of Bi-Mn alloys,” Journal of Crystal Growth, Vol. 52, 519–523, 1981.
4. De Rango, P., M. Lees, P. Lejay, A. Sulpice, R. Tournier, M. Ingold, P. Germi, and M. Pernet, “Texturing of magnetic materials at high temperature by solidification in a magnetic field,”Nature, Vol. 349, 770–772, 1991.
5. Liu, H. B., P. J. Ferreira, and J. B. Vander Sande, “Processing 2212/ag thick films under a high magnetic field: On the bi-2212/ag interface effect,” Physica C: Superconductivity, Vol. 303, 161–168, 1998.
6. Gaucherand, F. and E. Beaugnon, “Magnetic texturing in ferromagnetic cobalt alloys,” Physica B, Vol. 346–347, 262–266, 2004.
8. Torbet, J., J. M. Freyssinet, and G. Hudry-Clergeon, “Oriented fibrin gels formed by polymerization in strong magnetic fields,”
Nature, Vol. 289, 91–93, 1981.
9. Tournier, R. F. and E. Beaugnon, “Texturing by cooling a metallic melt in a magnetic field,” Science and Technology of Advanced Materials, Vol. 10, 014501, 2009.
10. Tournier, R. F, “Presence of intrinsic growth nuclei in overheated and undercooled liquid elements,” Physica B, Vol. 392, 79–91, 2007.
11. Li, C. J., Z. M. Ren, K. Deng, G. H. Cao, Y. B. Zhong, and Y. Q. Wu, “Design and application of differential thermal analysis apparatus in high magnetic fields,” Review of Scientific Instruments, Vol. 80, 073907, 2009.
12. Porter, D. A. and K. E. Easterling, Phase Transformations in Metals and Alloys, 2nd Edition, Chapman & Hall, London, 1992. 13. Magomedov, M. N., “On the magnetic-field-induced changes in the parameters of phase transitions,” Technical Physics Letters, Vol. 28, 116–118, 2002.
14. Turnbull, D., “Formation of crystal nuclei in liquid metals,”
Journal of Applied Physics, Vol. 21, 1022–1028, 1950.
15. Fujimura, Y. and M. Lino, “The surface tension of water under high magnetic fields,” Journal of Applied Physics, Vol. 103, 124903-4, 2008.
16. Li, C. J., H. Yang, Z. M. Ren, W. L. Ren, and Y. Q. Wu, “On nucleation temperature of pure aluminum in magnetic fields,”
Progress In Electromagnetics Research Letters, Vol. 15, 45–52, 2010.
17. Spaepen, F., “Interfaces and stresses in thin films,” Acta Materialia, Vol. 48, 31–42, 2000.
18. Turnbull, D. and J. C. Fisher, “Rate of nucleation in condensed systems,”Journal of Chemical Physics, Vol. 17, 71–73, 1949. 19. Botton, V., P. Lehmann, R. Bolcato, R. Moreau, and R. Haettel,
“Measurement of solute diffusivities. Part II. Experimental measurements in a convection-controlled shear cell. Interest of a uniform magnetic field,”International Journal of Heat and Mass Transfer, Vol. 44, 3345–3357, 2001.
20. Miyake, T., Y. Inatomi, and K. Kuribayashi, “Measurement of diffusion coefficient in liquid metal under static magnetic field,”
Japan Journal of Applied Physics, Vol. 41, L811–L813, 2002. 21. Youdelis, W. V., D. R. Colton, and J. Cahoon, “On the theory
Vol. 42, No. 11, 2238–2258, 1964.
22. Ferreira, P. J., H. B. Liu, and J. B. Vander Sande, “A model for the texture development of high-Tc surperconductors under an elevated magnetic field,” Journal of Materials Research, Vol. 14, 2751–2763, 1999.
23. Asai, S., K. Sassa, and M. Tahashi, “Crystal orientation of non-magnetic materials by imposition of a high magnetic field,”
Science and Technology of Advanced Materials, Vol. 4, 455–460, 2003.
24. Sugiyama, T., M. Tahashi, K. Sassa, and S. Asai, “The control of crystal orientation in non-magnetic metals by imposition of a magnetic field,”ISIJ International, Vol. 43, 855–861, 2003. 25. Nakagawa, Y., “An experiment on the inhibition of thermal
convection by a magnetic field,”Nature, Vol. 175, 417–419, 1955. 26. Oreper, G. M. and J. Szekely, “The effect of an externally imposed magnetic field on buoyancy driven flow in a rectangular cavity,”
Journal of Crystal Growth, Vol. 64, 505–515, 1983.
27. Lehmann, P., R. Moreau, D. Camel, and R. Bolcato, “Modifi-cation of interdendritic convection in directional solidifi“Modifi-cation by a uniform magnetic field,” Acta Materialia, Vol. 46, 4067–4079, 1998.
28. Moreau, R., O. Laskar, M. Tanaka, and D. Camel, “Thermoelec-tric magnetohydrodynamic effects on solidification of metallic al-loys in the dendritic regime,” Materials Science and Engineering A, Vol. 173, 93–100, 1993.
29. Gorbunov, L. A., “Effect of thermoelectromagnetic convection on the production of bulk single crystals consisting of semiconductor melts in a constant magnetic field,” Magnetohydrodynamics, Vol. 23, 404–408, 1988.
30. Li, X., Y. Fautrelle, and Z. M. Ren, “Influence of thermoelectric effects on the solid–liquid interface shape and cellular morphology in the mushy zone during the directional solidification of Al-Cu alloys under a magnetic field,” Acta Materialia, Vol. 55, 3803– 3813, 2007.
31. Shercliff, J. A., “Thermoelectric magnetohydrodynamics,” Jour-nal of Fluid Mechanics, Vol. 91, 231–251, 1979.